- Aug 10, 2017 -
one of Method and use of frit recipe
1. Low temperature red frit
lead Dan 42% borax 1% boric acid 1.6 % zinc oxide 2.6% stalactite 11% quartz 26%
potash feldspar 10%
B. Preparation method: mineral raw materials first crushed 40 to 60 mesh sieve, and then add the chemical raw materials mixed evenly, into the bottom of the sag, with the oxidation of flame burning to 1230 ℃;Make it melt crushed, sieved, washed, dried spare
C. Use: with low temperature chicken blood red glaze
About ZiBo YiShun ceramic glaze:
Zibo Yishun ceramic pigment & glaze Co., Ltd is was founded in 1999. It is located in Zibo city, a Capital of Ceramics and the biggest manufacturing base of ceramics material. We are now promoting ceramics raw material worldwide and providing professional importing and exporting service. We as a manufacturer specializes in manufacturing various ceramic raw materials .Our main products include: various kinds of ceramic frit (transparent frit, inkjet frit, matt frit, water-proof titanium frit, opaque/zirconium white frit, lead frit, small and big C.O.E. frit ,frit powder), zinc oxide, alumina oxide, , CMC, kaolin, lithium china stone powder, feldspar , ceramic pigment (every kinds of color) and other chemical raw materials used in ceramic..
Yishun adheres to the belief of “customers first, forge ahead” and we will always provide the highest quality to our customers. Now Yishun’s products are popular in many cities and provinces in China, and even exported to Korea, Indonesia, India, Bulgaria, Vietnam and Chile, etc. We can offer you the most reliable quality, the most reasonable price, prompt delivery and excellent service before & after sale.
How to get the sample free of charge?
1.You can sent inquiry to our email: email@example.com
Whatsapp num:+86 13573523942
3.Cell number:+86 13573523942
Welcome to send inquiry! Send Now!